# Novel Van Der Waals Heterostructures Based on Borophene, Graphene-like GaN and ZnO for Nanoelectronics: A First Principles Study

^{1}

^{2}

^{*}

## Abstract

**:**

## 1. Introduction

_{2}and MoSe

_{2}, as well as WS

_{2}and WSe

_{2}[24,25,26,27,28]. Metal oxides, in particular zinc oxide and titanium dioxide, as well as third group semiconductor nitrides, such as gallium, aluminum, and indium nitride, are promising materials for creating UV radiation photodetectors [29]. Among the ways to implement UV radiation sensors, preference is given to detection devices based on photodiodes with a Schottky barrier [30,31,32,33] formed by a metal–semiconductor contact. Such contacts are predominantly fabricated on the basis of van der Waals heterostructures containing graphene. In particular, experimental and theoretical studies have been carried out for such van der Waals heterostructures as graphene/MoS

_{2}[34], graphene/boron nitride [35], graphene/InSe [36], MoTe

_{2}/MoS

_{2}[37], graphene/phosphorene, and heterostructures based on phosphorene and MoSe

_{2}allotropes [38].

_{2}N [45], borophene/MoSe

_{2}, and borophene/WSe

_{2}[46] have already been proposed.

## 2. Methods and Approaches

#### 2.1. Atomistic Models of van der Waals Heterostructures

_{x}= 3.204 Å and L

_{y}= 5.55 Å, and the initial translation vectors of the ZnO unit cell are L

_{x}= 3.205 Å and L

_{y}= 5.5516 Å. Among the allotropic forms of borophene, we chose a triangulated borophene (tr-B) with high energy stability and geometric features that allow it to be combined with GaN and ZnO monolayers [51]. The unit cell of tr-B is originally set by means of atomic positions obtained from the data reported by Peng et al. [52]. The translation vectors of the tr-B unit cell are L

_{x}= 1.613 Å; L

_{y}= 2.864 Å. The close match between the lattice parameters of tr-B and GaN (1.613 Å (3.226 Å) and 3.204 Å, respectively, mismatch ~1%), tr-B and ZnO (1.613 Å (3.226 Å) and 3.205 Å, respectively, mismatch ~1%) makes it possible to create layered heterostructures with minimal mechanical stresses in the plane of the structure. Figure 1 and Figure 2 show the process of overlaying 2D monolayers during the formation of atomistic models of tr-B/GaN and tr-B/ZnO heterostructures with expanded rectangular cells. The original supercell of the tr-B/GaN heterostructure is shown in Figure 1c. It has optimized translation vectors L

_{x}= 3.35 Å and L

_{y}= 6.105 Å. The extended fragment of the tr-B/GaN supercell (see Figure 1a) was obtained by a threefold increase in the vector L

_{x}and twofold increase in the vector L

_{y}of the original supercell. The original supercell of the tr-B/ZnO heterostructure is shown in Figure 2c. Its translation vectors are L

_{x}= 3.28 Å and L

_{y}= 5.83 Å. The extended fragment of the tr-B/ZnO supercell (see Figure 2a) was obtained similarly to an extended fragment of the tr-B/GaN supercell. The distance between the tr-B and GaN monolayers along the Z-axis was 2.91 Å (see Figure 1b), between the tr-B and ZnO monolayers were 2.51 Å (see Figure 2b).

_{b}per atom. The calculation was carried out according to the following equation:

_{tr-B/GaN(ZnO)}is the total energy of the tr-B/GaN (tr-B/ZnO) heterostructure, E

_{tr-B}is the total energy of the isolated layer of triangulated borophene, E

_{GaN(ZnO)}is the total energy of the isolated GaN(ZnO) monolayer, N is the number of atoms in the heterostructure. According to the calculation results, the binding energy for a tr-B/GaN supercell is ~−0.05 eV/atom, and for a tr-B/ZnO supercell, it is ~−0.08 eV/atom. The negative value of the binding energy indicates that the tr-B/GaN and tr-B/ZnO heterostructures are energetically stable and, therefore, can be implemented in practice. In addition, in terms of energy stability (value of binding energy), they are superior to a number of other heterostructures based on GaN and ZnO monolayers, for example, MoSSe-g-GaN and WSSe-g-GaN heterostructures by almost two times [53], and ZnO/g-GeC heterostructures by more than six times [54].

#### 2.2. Calculation Details

_{b}is the bias voltage, e is the electron charge, h is Planck′s constant, f(E-μ

_{L/R}) are the Fermi–Dirac distribution functions for the left (L) and right (R) electrodes, respectively, μ

_{L/R}= E

_{F}± V

_{b}/2 is the chemical potential of the left (L) and right (R) electrodes, which shifted upwards (downwards) relative to the Fermi energy E

_{F}, T(E,V

_{b}) is the quantum mechanical probability of electrons passing through the channel (transmission coefficient), which can be expressed as follows

_{b}), G

^{†}(E,V

_{b}) are the retarded and advanced Green′s functions describing the contact with the electrodes, Γ

_{L}(E), Γ

_{D}(E) are the level broadening matrices for the left (L) and right (R) electrode. Level broadening matrices for each of the electrodes are defined as

_{L/R}are the self-energy matrices of the left (L) and right (R) electrodes. Green′s matrices are calculated as:

_{C}is the overlap matrix of atomic orbitals of the conducting channel, E is the electron energy; H

_{C}is the Hamiltonian of the conducting channel.

## 3. Results and Discussion

#### 3.1. Electronic Structure of tr-B/GaN and tr-B/ZnO Heterostructures

_{x}(Г–X, S–Y, Г–S). A linear dispersion relation is observed along the Г–X, S–Y, and Г–S paths, which is characteristic of triangulated borophene (Figure 4b). Consequently, the GaN monolayer, which plays the role of a kind of substrate for borophene, does not make a decisive contribution to the electronic structure of the tr-B/GaN heterostructure. In the k

_{y}direction (X–S, Y–Г), the energy bands near the top of the valence band and the bottom of the conduction band are flat, which corresponds to a larger effective mass of charge carriers in this direction. Near the top of the valence band in Г–X, S–Y, Г–S paths, the dispersion law is close to isotropic parabolic, which is typical for the energy bands near the top of the valence band of GaN (Figure 4c). On the whole, the presence of band dispersion anisotropy in the electronic structure of tr-B/GaN should be noted.

_{x}direction) and Г–S paths. Interestingly, the linear dispersion relation is typical for borophene in the entire k

_{x}direction (Г–X, S–Y, and Г–S, see Figure 6b), while for the tr-B/ZnO heterostructure it mainly has a place in the G–X path, both near the bottom of the conduction band and near the top of the valence band. In the S–Y and Г–S paths, the linear dispersion relation is observed only at the bottom of the conduction band, while in the valence band there is a tendency to transition from a linear dispersion relation to a parabolic one, and hence to a nonzero effective mass.

#### 3.2. Electrical Properties of tr-B/GaN and tr-B/ZnO Heterostructures

_{12}/MoS

_{2}[46], SeMoS/SMoS, and SMoSe/SMoS [67] van der Waals heterostructures used as a Schottky contact. The comparison results showed that at the same voltages, the current values in the β

_{12}/MoS

_{2}MoS

_{2}/WSe

_{2}/graphene, SeMoS/SMoS, and SMoSe/SMoS heterostructures are no more than a few nanoamperes, while the current values in the tr-B heterostructures/GaN and tr-B/ZnO is measured in tens of microamperes. In addition, the β

_{12}/MoS

_{2}heterostructure in terms of binding energy is two times inferior to the tr-B/GaN heterostructure and three times inferior to the tr-B/ZnO heterostructure. Therefore, it can be predicted that tr-B/GaN and tr-B/ZnO van der Waals heterostructures can also be competitive as Schottky barriers for use in various nano- and optoelectronic devices.

## 4. Conclusions

## Author Contributions

## Funding

## Institutional Review Board Statement

## Informed Consent Statement

## Data Availability Statement

## Conflicts of Interest

## References

- Novoselov, K.S.; Geim, A.K.; Morozov, S.V.; Jiang, D.; Zhang, Y.; Dubonos, S.V.; Grigorieva, I.V.; Firsov, A.A. Electric field effect in atomically thin carbon films. Science
**2004**, 306, 666–669. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Mas-Ballesté, R.; Gómez-Navarro, C.; Gómez-Herrero, J.; Zamora, F. 2D materials: To graphene and beyond. Nanoscale
**2011**, 3, 20–30. [Google Scholar] [CrossRef] [PubMed] - Xu, M.; Liang, T.; Shi, M.; Chen, H. Graphene-Like Two-Dimensional Materials. Chem. Rev.
**2013**, 113, 3766–3798. [Google Scholar] [CrossRef] [PubMed] - Bhimanapati, G.R.; Lin, Z.; Meunier, V.; Jung, Y.; Cha, J.; Das, S.; Xiao, D.; Son, Y.; Strano, M.; Cooper, V.; et al. Recent Advances in Two-Dimensional Materials beyond Graphene. ACS Nano
**2015**, 9, 11509–11539. [Google Scholar] [CrossRef] - Miró, P.; Audiffred, M.; Heine, T. An atlas of two-dimensional materials. Chem. Soc. Rev.
**2014**, 43, 6537–6554. [Google Scholar] [CrossRef] - Kong, X.; Liu, Q.; Zhang, C.; Peng, Z.; Chen, Q. Elemental two-dimensional nanosheets beyond graphene. Chem. Soc. Rev.
**2017**, 46, 2127–2157. [Google Scholar] [CrossRef] - Xia, F.; Wang, H.; Xiao, D.; Dubey, M.; Ramasubramaniam, A. Two-dimensional material nanophotonics. Nat. Photonics
**2014**, 8, 899–907. [Google Scholar] [CrossRef] - Khan, K.; Tareen, A.; Aslam, M.; Wang, R.; Zhang, Y.; Mahmood, A.; Ouyang, Z.; Han, Z.; Guo, Z. Recent developments in emerging two-dimensional materials and their applications. J. Mater. Chem. C
**2020**, 8, 387–440. [Google Scholar] [CrossRef] - Chen, J.; He, X.; Sa, B.; Zhou, J.; Xu, C.; Wen, C.; Sun, Z. III–VI van der Waals heterostructures for sustainable energy related applications. Nanoscale
**2019**, 11, 6431–6444. [Google Scholar] [CrossRef] - Geim, A.K.; Grigorieva, I.V. Van der Waals heterostructures. Nature
**2013**, 499, 419–425. [Google Scholar] [CrossRef] - Novoselov, K.S.; Mishchenko, A.; Carvalho, A.; Castro Neto, A.H. 2D materials and van der Waals heterostructures. Science
**2016**, 353, aac9439. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Liu, Y.; Weiss, N.O.; Duan, X.; Cheng, H.-C.; Huang, Y.; Duan, X. Van der Waals heterostructures and devices. Nat. Rev. Mater.
**2016**, 1, 16042. [Google Scholar] [CrossRef] - Zhong, D.; Seyler, K.L.; Linpeng, X.; Cheng, R.; Sivadas, N.; Huang, B.; Schmidgall, E.; Taniguchi, T.; Watanabe, K.; McGuire, M.A.; et al. Van der Waals engineering of ferromagnetic semiconductor heterostructures for spin and valleytronics. Sci. Adv.
**2017**, 3, e1603113. [Google Scholar] [CrossRef] [Green Version] - Unuchek, D.; Ciarrocchi, A.; Avsar, A.; Watanabe, K.; Taniguchi, T.; Kis, A. Room-temperature electrical control of exciton flux in a van der Waals heterostructure. Nature
**2018**, 560, 340–344. [Google Scholar] [CrossRef] - Wang, Y.; Liu, E.; Gao, A.; Cao, T.; Long, M.; Pan, C.; Zhang, L.; Zeng, J.; Wang, C.; Hu, W.; et al. Negative Photoconductance in van der Waals Heterostructure-Based Floating Gate Phototransistor. ACS Nano
**2018**, 12, 9513–9520. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Zhou, X.; Hu, X.; Yu, J.; Liu, S.; Shu, Z.; Zhang, Q.; Li, H.; Ma, Y.; Xu, H.; Zhai, T. 2D Layered Material-Based van der Waals Heterostructures for Optoelectronics. Adv. Funct. Mater.
**2018**, 28, 1706587. [Google Scholar] [CrossRef] - Liang, S.; Cheng, B.; Cui, X.; Miao, F. Van der Waals Heterostructures for High-Performance Device Applications: Challenges and Opportunities. Adv. Mater.
**2019**, 32, 1903800. [Google Scholar] [CrossRef] [Green Version] - Georgiou, T.; Jalil, R.; Belle, B.D.; Britnell, L.; Gorbachev, R.V.; Morozov, S.V.; Kim, Y.J.; Gholinia, A.; Haigh, S.J.; Makarovsky, O.; et al. Vertical field-effect transistor based on graphene-WS
_{2}heterostructures for flexible and transparent electronics. Nat. Nanotechnol.**2013**, 8, 100–103. [Google Scholar] [CrossRef] - Liu, X.; Qu, D.; Li, H.M.; Moon, I.; Ahmed, F.; Kim, C.; Lee, M.; Choi, Y.; Cho, J.H.; Hone, J.C.; et al. Modulation of Quantum Tunneling via a Vertical Two-Dimensional Black Phosphorus and Molybdenum Disulfide p-n Junction. ACS Nano
**2017**, 11, 9143–9150. [Google Scholar] [CrossRef] - Yan, X.; Liu, C.; Li, C.; Bao, W.; Ding, S.; Zhang, D.W.; Zhou, P. Tunable SnSe
_{2}/WSe_{2}heterostructure tunneling field effect transistor. Small**2017**, 13, 1701478. [Google Scholar] [CrossRef] - Zubair, A.; Nourbakhsh, A.; Hong, J.Y.; Qi, M.; Song, Y.; Jena, D.; Kong, J.; Dresselhaus, M.; Palacios, T. Hot Electron Transistor with van der Waals Base-Collector Heterojunction and High-Performance GaN Emitter. Nano Lett.
**2017**, 17, 3089–3096. [Google Scholar] [CrossRef] [PubMed] - Vaziri, S.; Lupina, G.; Henkel, C.; Smith, A.D.; Ostling, M.; Dabrowski, J.; Lippert, G.; Mehr, W.; Lemme, M.C. A graphene-based hot electron transistor. Nano Lett.
**2013**, 13, 1435–1439. [Google Scholar] [CrossRef] [PubMed] - Song, T.; Cai, X.; Tu, M.W.; Zhang, X.; Huang, B.; Wilson, N.P.; Seyler, K.L.; Zhu, L.; Taniguchi, T.; Watanabe, K.; et al. Giant tunneling magnetoresistance in spin-filter van der Waals heterostructures. Science
**2018**, 360, 1214–1218. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Bellus, M.Z.; Li, M.; Lane, S.D.; Ceballos, F.; Cui, Q.; Zeng, X.C.; Zhao, H. Type-I van der Waals heterostructure formed by MoS
_{2}and ReS_{2}monolayers. Nanoscale Horiz.**2017**, 2, 31–36. [Google Scholar] [CrossRef] - Hong, X.; Kim, J.; Shi, S.; Zhang, Y.; Jin, C.; Sun, Y.; Tongay, S.; Wu, J.; Zhang, Y.; Wang, F. Ultrafast charge transfer in atomically thin MoS
_{2}/WS_{2}heterostructures. Nat. Nanotech.**2014**, 9, 682–686. [Google Scholar] [CrossRef] [Green Version] - Gong, Y.; Lin, J.; Wang, X.; Shi, G.; Lei, S.; Lin, Z.; Zou, X.; Ye, G.; Vajtai, R.; Yakobson, B.; et al. Vertical and in-plane heterostructures from WS
_{2}/MoS_{2}monolayers. Nat. Mater.**2014**, 13, 1135–1142. [Google Scholar] [CrossRef] [Green Version] - Yu, Y.; Hu, S.; Su, L.; Huang, L.; Liu, Y.; Jin, Z.; Purezky, A.; Geohegan, D.; Kim, K.; Zhang, Y.; et al. Equally Efficient Interlayer Exciton Relaxation and Improved Absorption in Epitaxial and Nonepitaxial MoS
_{2}/WS_{2}Heterostructures. Nano Lett.**2015**, 15, 486–491. [Google Scholar] [CrossRef] [Green Version] - Yuan, J.; Najmaei, S.; Zhang, Z.; Zhang, J.; Lei, S.; Ajayan, P.M.; Yakobson, B.; Lou, J. Photoluminescence Quenching and Charge Transfer in Artificial Heterostacks of Monolayer Transition Metal Dichalcogenides and Few-Layer Black Phosphorus. ACS Nano
**2015**, 9, 555–563. [Google Scholar] [CrossRef] - Zou, Y.; Zhang, Y.; Hu, Y.; Gu, H. Ultraviolet Detectors Based on Wide Bandgap Semiconductor Nanowire: A Review. Sensors
**2018**, 18, 2072. [Google Scholar] [CrossRef] [Green Version] - Peng, L.; Cui, Y.; Sun, L.; Du, J.; Wang, S.; Zhang, S.; Huang, Y. Dipole controlled Schottky barrier in the blue-phosphorene-phase of GeSe based van der Waals heterostructures. Nanoscale Horiz.
**2019**, 4, 480–489. [Google Scholar] [CrossRef] - Zhang, W.X.; Yina, Y.; He, C. Lowering the Schottky barrier height of G/WSSe van der Waals heterostructures by changing the interlayer coupling and applying external biaxial strain. Phys. Chem. Chem. Phys.
**2020**, 22, 26231–26240. [Google Scholar] [CrossRef] [PubMed] - Zhu, Y.; Liu, K.; Ai, Q.; Hou, Q.; Chen, X.; Zhang, Z.; Xie, X.; Lia, B.; Shen, D. A high performance self-powered ultraviolet photodetector based on a p-GaN/n-ZnMgO heterojunction. J. Mater. Chem. C
**2020**, 8, 2719–2724. [Google Scholar] [CrossRef] - Liu, Z.; Wang, X.; Liu, Y.; Guo, D.; Li, S.; Yan, Z.; Tan, C.-K.; Li, W.; Li, P.; Tang, W. A high-performance ultraviolet solar-blind photodetector based on a β-Ga
_{2}O_{3}Schottky photodiode. J. Mater. Chem. C**2019**, 7, 13920–13929. [Google Scholar] [CrossRef] - Yu, L.; Lee, Y.H.; Ling, X.; Santos, E.J.; Shin, Y.C.; Lin, Y.; Dubey, M.; Kaxiras, E.; Kong, J.; Wang, H.; et al. Graphene/MoS
_{2}hybrid technology for large-scale two-dimensional electronics. Nano Lett.**2014**, 14, 3055–3063. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Wang, J.; Ma, F.; Sun, M. Graphene, hexagonal boron nitride, and their heterostructures: Properties and applications. RSC Adv.
**2017**, 7, 16801–16822. [Google Scholar] [CrossRef] [Green Version] - Mudd, G.W.; Svatek, S.A.; Hague, L.; Makarovsky, O.; Kudrynsky, Z.R.; Mellor, C.J.; Beton, P.H.; Eaves, L.; Novoselov, K.S.; Kovalyuk, Z.D.; et al. High broad-band photoresponsivity of mechanically formed InSe graphene van der Waals heterostructures. Adv. Mater.
**2015**, 27, 3760–3766. [Google Scholar] [CrossRef] [Green Version] - Zhang, K.; Zhang, T.; Cheng, G.; Li, T.; Wang, S.; Wei, W.; Zhou, X.; Yu, W.; Sun, Y.; Wang, P.; et al. Interlayer Transition and Infrared Photodetection in Atomically Thin Type-II MoTe
_{2}/MoS_{2}van der Waals Heterostructures. ACS Nano**2016**, 10, 3852–3858. [Google Scholar] [CrossRef] - Kaur, S.; Kumar, A.; Srivastava, S.; Tankeshwar, K. van der Waals heterostructures based on allotropes of phosphorene and MoSe
_{2}. Phys. Chem. Chem. Phys.**2017**, 19, 22023–22032. [Google Scholar] [CrossRef] [Green Version] - Mannix, A.J.; Zhou, X.-F.; Kiraly, B.; Wood, J.D.; Alducin, D.; Myers, B.D.; Liu, X.; Fisher, B.L.; Santiago, U.; Guest, J.R.; et al. Synthesis of borophenes: Anisotropic, two-dimensional boron polymorphs. Science
**2015**, 350, 1513–1516. [Google Scholar] [CrossRef] [Green Version] - Shen, J.; Yang, Z.; Wang, Y.; Xu, L.-C.; Liu, R.; Liu, X. Organic Gas Sensing Performance of the Borophene van der Waals Heterostructure. J. Phys. Chem. C
**2021**, 125, 427–435. [Google Scholar] [CrossRef] - Huo, Y.; Liu, R.; Sun, Q.; Yang, Z.; Xu, L.-C.; Liu., X. Inorganic gas sensing performance of χ3-borophene and the van der Waals heterostructure. Appl. Surf. Sci.
**2022**, 581, 151906. [Google Scholar] [CrossRef] - Cuxart, M.G.; Seufert, K.; Chesnyak, V.; Waqas, W.A.; Robert, A.; Bocquet, M.L.; Duesberg, G.S.; Sachdev, H.; Auwärter, W. Borophenes made easy. Sci. Adv.
**2021**, 7, eabk1490. [Google Scholar] [CrossRef] [PubMed] - Hou, C.; Tai, G.; Liu, B.; Wu, Z.; Yin, Y. Borophene-graphene heterostructure: Preparation and ultrasensitive humidity sensing. Nano Res.
**2021**, 14, 2337–2344. [Google Scholar] [CrossRef] - Jing, S.; Chen, W.; Pan, J.; Li, W.; Bian, B.; Liao, B.; Wang, G. Electronic properties of Borophene/InSe van der Waals heterostructures. Mater. Sci. Semicond. Process.
**2022**, 146, 106673. [Google Scholar] [CrossRef] - Jiang, J.W.; Wang, X.C.; Song, Y.; Mi, W.B. Tunable Schottky Barrier and Electronic Properties in Borophene/g-C
_{2}N van der Waals Heterostructures. Appl. Surf. Sci.**2018**, 440, 42–46. [Google Scholar] [CrossRef] - Katoch, N.; Kumar, A.; Sharma, R.; Ahluwalia, P.K.; Kumar, J. Strain Tunable Schottky Barriers and Tunneling Characteristics of Borophene/MX2 van der Waals Heterostructures. Phys. E Low-Dimens. Syst. Nanostructures
**2020**, 120, 113842. [Google Scholar] [CrossRef] - Wu, Z.; Li, X.; Zhong, H.; Zhang, S.; Wang, P.; Kim, T.H.; Kwak, S.S.; Liu, C.; Chen, H.; Kim, S.W.; et al. Graphene/h-BN/ZnO van der Waals tunneling heterostructure based ultraviolet photodetector. Opt. Express
**2015**, 23, 18864–18871. [Google Scholar] [CrossRef] [Green Version] - Lin, F.; Liao, X.; Liu, C.P.; Zhang, Z.S.; Liu, S.; Yu, D.; Liao, Z.M. Graphene/ZnO Nanowire/p-GaN Vertical Junction for a High-Performance Nanoscale Light Source. ACS Omega
**2020**, 8, 4133–4138. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Wu, J.; Gong, M. ZnO/graphene heterostructure nanohybrids for optoelectronics and sensors. J. Appl. Phys.
**2021**, 130, 070905. [Google Scholar] [CrossRef] - The Materials Project. Available online: https://materialsproject.org/ (accessed on 4 February 2022).
- Xie, Z.; Meng, X.; Li, X.; Liang, W.; Huang, W.; Chen, K.; Chen, J.; Xing, C.; Qiu, M.; Zhang, B.; et al. Two-Dimensional Borophene: Properties, Fabrication, and Promising Applications. Research
**2020**, 2020, 2624617. [Google Scholar] [CrossRef] [PubMed] - Peng, B.; Zhang, H.; Shao, H.; Ning, Z.; Xu, Y.; Ni, G.; Lu, H.; Zhang, D.; Zhu, H. Stability and strength of atomically thin borophene from first principles calculations. Mater. Res. Lett.
**2017**, 5, 399–407. [Google Scholar] [CrossRef] - Idrees, M.; Nguyen, C.V.; Bui, H.D.; Ahmad, I.; Amin, B. Van der Waals heterostructures based on MSSe (M = Mo, W) and graphene-like GaN: Enhanced optoelectronic and photocatalytic properties for water splitting. Phys. Chem. Chem. Phys.
**2020**, 22, 20704–20711. [Google Scholar] [CrossRef] [PubMed] - Gao, X.; Shen, Y.; Ma, Y.; Wu, S.; Zhou, Z. ZnO/g-GeC van der Waals heterostructure: Novel photocatalyst for small molecule splitting. J. Mater. Chem. C
**2019**, 7, 4791–4799. [Google Scholar] [CrossRef] - Soler, J.M.; Artacho, E.; Gale, J.D.; García, A.; Junquera, J.; Ordejón, P.; Sánchez-Portal, D. The SIESTA method for ab-initio order-N materials simulation. J. Phys. Condens. Matter
**2002**, 14, 2745–2779. [Google Scholar] [CrossRef] [Green Version] - The SIESTA Group. Available online: Departments.icmab.es/leem/siesta/ (accessed on 10 December 2021).
- García, A.; Papior, N.; Akhtar, A.; Artacho, E.; Blum, V.; Bosoni, E.; Brandimarte, P.; Brandbyge, M.; Cerdá, J.I.; Corsetti, F.; et al. Siesta: Recent developments and applications. J. Chem. Phys.
**2020**, 152, 204108. [Google Scholar] [CrossRef] - Perdew, J.P.; Chevary, J.A.; Vosko, S.H.; Jackson, K.A.; Pederson, M.R.; Singh, D.J.; Fiolhais, C. Atoms, molecules, solids, and surfaces: Applications of the generalized gradient approximation for exchange and correlation. Phys. Rev. B
**1992**, 46, 6671–6687. [Google Scholar] [CrossRef] - Grimme, S. Semiempirical GGA-type Density Functional Constructed with a Long-Range Dispersion Correction. J. Comput. Chem.
**2006**, 27, 1787–1799. [Google Scholar] [CrossRef] - Monkhorst, H.J.; Pack, J.D. Special points for Brillouin-zone integrations. Phys. Rev. B
**1976**, 13, 5188–5192. [Google Scholar] [CrossRef] - Pulay, P. Convergence acceleration of iterative sequences. The case of SCF iteration. Chem. Phys. Lett.
**1980**, 73, 393–398. [Google Scholar] [CrossRef] - Brandbyge, M.; Mozos, J.-L.; Ordejón, P.; Taylor, J.; Stokbro, K. Density-functional method for nonequilibrium electron transport. Phys. Rev. B
**2002**, 65, 165401. [Google Scholar] [CrossRef] [Green Version] - Mozos, J.L.; Ordejón, P.; Brandbyge, M.; Taylor, J.; Stokbro, K. Simulations of quantum transport in nanoscale systems: Application to atomic gold and silver wires. Nanotechnology
**2002**, 13, 346–351. [Google Scholar] [CrossRef] - Büttiker, M.; Imry, Y.; Landauer, R.; Pinhas, S. Generalized Many-Channel Conductance Formula with Application to Small Rings. Phys. Rev. B
**1985**, 31, 6207–6215. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Datta, S. Quantum Transport: Atom to Transistor, 2nd ed.; Cambridge University Press: New York, NY, USA, 2005; pp. 217–249. [Google Scholar]
- Lu, H.; Dai, D.; Yanga, P.; Lic, L. Atomic orbitals in molecules: General electronegativity and improvement of Mulliken population analysis. Phys. Chem. Chem. Phys.
**2006**, 8, 340–346. [Google Scholar] [CrossRef] [PubMed] - Liu, J.; Ren, J.C.; Shen, T.; Liu, X.; Butch, C.J.; Li, S.; Liu, W. Asymmetric Schottky Contacts in van der Waals Metal-Semiconductor-Metal Structures Based on Two-Dimensional Janus Materials. Research
**2020**, 2020, 6727524. [Google Scholar] [CrossRef] [PubMed]

**Figure 1.**The process of constructing atomistic models of van der Waals tr-B/GaN heterostructure: top view (

**a**) and side view (

**b**) of an extended supercell fragment; the original supercell of tr-B/GaN heterostructure (

**c**) marked with a red box in (

**a**).

**Figure 2.**The process of constructing atomistic models of van der Waals tr-B/ZnO heterostructures: top view (

**a**) and side view (

**b**) of an extended supercell fragment; the original supercell of tr-B/ZnO heterostructure (

**c**) marked with a red box in (

**a**).

**Figure 3.**Schematic representation of a conducting channel (scattering region) enclosed between two electrodes as part of tr-B/GaN and tr-B/ZnO vertical heterostructures for current transfer along the zigzag (

**a**) and armchair directions (

**b**) of GaN/ZnO monolayer.

**Figure 4.**Band structure of the tr-B/GaN van der Waals heterostructure (

**a**) and its constituent monolayers of triangulated borophene tr-B (

**b**) and gallium nitride GaN (

**c**). In (

**a**), the top of the valence band is highlighted in red, and the bottom of the conduction band is highlighted in blue.

**Figure 6.**Band structure of the tr-B/ZnO van der Waals heterostructure (

**a**) and its constituent monolayers of triangulated borophene tr-B (

**b**) and zinc oxide ZnO (

**c**). In (

**a**), the top of the valence band is highlighted in red, and the bottom of the conduction band is highlighted in blue and green.

**Figure 8.**I–V curves of the tr-B/GaN heterostructure for current transfer along the armchair (

**a**) and zigzag (

**b**) edges of a GaN monolayer.

**Figure 9.**I–V curves of the tr-B/ZnO heterostructure for current transfer along the armchair (

**a**) and zigzag (

**b**) edges of a ZnO monolayer.

**Figure 10.**Transmission coefficient T(E) in the cases of current transfer along the zigzag and armchair directions for (

**a**) tr-B/GaN and (

**b**) tr-B/ZnO heterostructures.

Publisher’s Note: MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations. |

© 2022 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Slepchenkov, M.M.; Kolosov, D.A.; Glukhova, O.E.
Novel Van Der Waals Heterostructures Based on Borophene, Graphene-like GaN and ZnO for Nanoelectronics: A First Principles Study. *Materials* **2022**, *15*, 4084.
https://doi.org/10.3390/ma15124084

**AMA Style**

Slepchenkov MM, Kolosov DA, Glukhova OE.
Novel Van Der Waals Heterostructures Based on Borophene, Graphene-like GaN and ZnO for Nanoelectronics: A First Principles Study. *Materials*. 2022; 15(12):4084.
https://doi.org/10.3390/ma15124084

**Chicago/Turabian Style**

Slepchenkov, Michael M., Dmitry A. Kolosov, and Olga E. Glukhova.
2022. "Novel Van Der Waals Heterostructures Based on Borophene, Graphene-like GaN and ZnO for Nanoelectronics: A First Principles Study" *Materials* 15, no. 12: 4084.
https://doi.org/10.3390/ma15124084